#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/86/4508618.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4508618
loop_
_publ_author_name
'Wang, Jing-Ping'
'Duan, Xian-Ying'
'Du, Xiao-Di'
'Niu, Jing-Yang'
_publ_section_title
;
 Novel Rare Earth Germanotungstates and Organic Hybrid
 Derivatives:  Synthesis and Structures of M/[α-GeW11O39] (M = Nd,
 Sm, Y, Yb) and Sm/[α-GeW11O39](DMSO)
;
_journal_issue                   10
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              2266
_journal_paper_doi               10.1021/cg050321s
_journal_volume                  6
_journal_year                    2006
_chemical_formula_sum            'C8 H43.5 Ge N2 Nd1.5 O48 W11'
_chemical_formula_weight         3247.25
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 105.75(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   18.846(4)
_cell_length_b                   13.443(3)
_cell_length_c                   27.561(6)
_cell_measurement_temperature    293(2)
_cell_volume                     6720(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.934
_diffrn_measured_fraction_theta_max 0.934
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0419
_diffrn_reflns_av_sigmaI/netI    0.0575
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            19527
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.52
_exptl_absorpt_coefficient_mu    20.401
_exptl_absorpt_correction_T_max  0.1933
_exptl_absorpt_correction_T_min  0.1126
_exptl_crystal_density_diffrn    3.210
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             5702
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.14
_exptl_crystal_size_min          0.12
_refine_diff_density_max         2.448
_refine_diff_density_min         -2.168
_refine_diff_density_rms         0.427
_refine_ls_extinction_coef       0.000230(17)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.079
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     722
_refine_ls_number_reflns         11053
_refine_ls_number_restraints     90
_refine_ls_restrained_S_all      1.075
_refine_ls_R_factor_all          0.0715
_refine_ls_R_factor_gt           0.0546
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0909P)²+10.5544P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1368
_refine_ls_wR_factor_ref         0.1445
_reflns_number_gt                9455
_reflns_number_total             11053
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg050321ssup1.cif
_cod_data_source_block           njy1
_cod_original_cell_volume        6720(2)
_cod_original_formula_sum        'C8 H43.50 Ge N2 Nd1.50 O48 W11'
_cod_database_code               4508618
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Nd1 Nd 0.27411(5) 0.18661(6) 0.74305(3) 0.0263(2) Uani 1 1 d .
Nd2 Nd 0.58551(17) 0.4746(2) 0.80169(9) 0.0754(9) Uani 0.50 1 d PU
Ge1 Ge 0.28679(9) 0.25411(10) 0.59432(5) 0.0215(3) Uani 1 1 d .
W1 W 0.45306(4) 0.37052(5) 0.57784(3) 0.03163(18) Uani 1 1 d .
W2 W 0.44176(4) 0.30901(5) 0.69591(2) 0.02740(17) Uani 1 1 d .
W3 W 0.45786(4) 0.13069(5) 0.61408(3) 0.02870(17) Uani 1 1 d .
W4 W 0.26853(4) 0.45115(4) 0.67203(2) 0.02477(17) Uani 1 1 d .
W5 W 0.12578(4) 0.40253(5) 0.57128(2) 0.02905(18) Uani 1 1 d .
W6 W 0.27700(4) 0.51286(5) 0.55410(3) 0.03362(19) Uani 1 1 d .
W7 W 0.29530(4) 0.30687(5) 0.46763(2) 0.03417(19) Uani 1 1 d .
W8 W 0.30037(4) 0.06817(5) 0.50599(2) 0.03122(18) Uani 1 1 d .
W9 W 0.14346(4) 0.19715(5) 0.48589(2) 0.03207(18) Uani 1 1 d .
W10 W 0.28996(4) 0.01188(4) 0.63909(2) 0.02587(17) Uani 1 1 d .
W11 W 0.13298(4) 0.13834(5) 0.61845(2) 0.02759(17) Uani 1 1 d .
O1 O 0.5181(7) 0.4370(8) 0.5575(5) 0.044(3) Uani 1 1 d .
O2 O 0.5045(7) 0.3543(9) 0.7490(5) 0.041(3) Uani 1 1 d .
O3 O 0.5275(7) 0.0455(8) 0.6202(5) 0.039(3) Uani 1 1 d .
O4 O 0.2740(6) 0.5417(8) 0.7186(4) 0.031(3) Uani 1 1 d .
O5 O 0.0365(7) 0.4452(8) 0.5572(5) 0.040(3) Uani 1 1 d .
O6 O 0.2858(8) 0.6226(9) 0.5256(5) 0.049(3) Uani 1 1 d .
O7 O 0.3104(8) 0.3528(10) 0.4140(5) 0.053(4) Uani 1 1 d .
O8 O 0.3196(8) -0.0377(8) 0.4769(5) 0.047(3) Uani 1 1 d .
O9 O 0.0597(8) 0.1743(10) 0.4426(5) 0.057(4) Uani 1 1 d .
O10 O 0.3038(6) -0.1148(7) 0.6396(4) 0.031(3) Uani 1 1 d .
O11 O 0.0428(7) 0.0962(8) 0.6041(5) 0.039(3) Uani 1 1 d .
O12 O 0.1335(6) 0.1398(7) 0.5427(4) 0.030(3) Uani 1 1 d .
O13 O 0.1970(7) 0.0821(8) 0.4707(4) 0.037(3) Uani 1 1 d .
O14 O 0.4875(7) 0.3887(8) 0.6479(5) 0.039(3) Uani 1 1 d .
O15 O 0.1252(7) 0.3235(8) 0.5136(4) 0.034(3) Uani 1 1 d .
O16 O 0.1636(6) 0.4695(7) 0.6349(4) 0.028(2) Uani 1 1 d .
O17 O 0.1197(6) 0.2803(8) 0.6046(4) 0.033(3) Uani 1 1 d .
O18 O 0.3775(7) 0.4668(7) 0.5742(4) 0.033(3) Uani 1 1 d .
O19 O 0.3901(6) 0.3213(7) 0.5150(4) 0.033(3) Uani 1 1 d .
O20 O 0.4947(6) 0.1976(8) 0.6781(4) 0.032(3) Uani 1 1 d .
O21 O 0.3703(7) 0.4163(8) 0.6828(4) 0.033(3) Uani 1 1 d .
O22 O 0.3194(7) 0.1697(8) 0.4587(4) 0.035(3) Uani 1 1 d .
O23 O 0.1917(7) 0.2718(9) 0.4429(4) 0.038(3) Uani 1 1 d .
O24 O 0.2852(6) 0.5521(7) 0.6198(4) 0.032(3) Uani 1 1 d .
O25 O 0.2782(6) 0.0228(8) 0.5617(4) 0.030(3) Uani 1 1 d .
O26 O 0.2669(7) 0.4212(8) 0.4983(4) 0.041(3) Uani 1 1 d .
O27 O 0.5004(7) 0.2397(8) 0.5852(4) 0.036(3) Uani 1 1 d .
O28 O 0.1723(7) 0.5061(7) 0.5410(4) 0.032(3) Uani 1 1 d .
O29 O 0.1839(7) 0.0131(7) 0.6211(4) 0.032(3) Uani 1 1 d .
O30 O 0.3872(6) 0.0624(7) 0.6393(4) 0.031(3) Uani 1 1 d .
O31 O 0.3963(6) 0.0999(8) 0.5471(4) 0.032(3) Uani 1 1 d .
O32 O 0.3829(6) 0.2339(7) 0.7204(4) 0.031(3) Uani 1 1 d .
O33 O 0.2463(7) 0.3413(8) 0.6995(4) 0.033(3) Uani 1 1 d .
O34 O 0.3013(6) 0.0358(7) 0.7036(4) 0.030(3) Uani 1 1 d .
O35 O 0.1529(6) 0.1526(8) 0.6852(4) 0.030(3) Uani 1 1 d .
O36 O 0.2505(6) 0.3721(7) 0.5981(4) 0.024(2) Uani 1 1 d .
O37 O 0.2642(6) 0.2206(7) 0.5310(4) 0.024(2) Uani 1 1 d .
O38 O 0.3825(6) 0.2637(7) 0.6157(4) 0.025(2) Uani 1 1 d .
O39 O 0.2534(6) 0.1702(7) 0.6303(4) 0.025(2) Uani 1 1 d .
O1W O 0.1737(15) 0.2518(18) 0.7802(12) 0.038(7) Uani 0.50 1 d P
O1W' O 0.2051(16) 0.227(2) 0.8049(12) 0.046(7) Uani 0.50 1 d P
O2W O 0.3302(9) 0.3424(11) 0.8016(6) 0.063(4) Uani 1 1 d .
O3W O 0.3721(8) 0.1328(10) 0.8179(5) 0.061(4) Uani 1 1 d .
O4W O 0.565(4) 0.553(5) 0.717(3) 0.058(17) Uani 0.25 1 d PU
O4W' O 0.579(4) 0.502(4) 0.7132(17) 0.051(17) Uani 0.25 1 d P
O5W O 0.607(2) 0.525(2) 0.8873(12) 0.092(13) Uani 0.50 1 d P
O6W O 0.4529(14) 0.5598(18) 0.7733(10) 0.044(6) Uani 0.50 1 d PU
O7W O 0.4868(19) 0.391(3) 0.8443(11) 0.0758(16) Uani 0.50 1 d PU
O8W O 0.669(2) 0.368(3) 0.7744(14) 0.081(10) Uani 0.50 1 d PU
O9W O 0.627(2) 0.292(3) 0.8404(15) 0.090(11) Uani 0.50 1 d PU
O10W O 1.421(2) 0.868(2) 0.7928(14) 0.086(12) Uani 0.50 1 d P
O11W O 1.0711(19) 1.133(2) 0.8269(12) 0.075(11) Uani 0.50 1 d P
O12W O 1.5872(11) 1.0378(13) 0.9238(7) 0.088(6) Uani 1 1 d .
O13W O 1.482(2) 1.009(3) 0.7515(14) 0.081(10) Uani 0.50 1 d P
O14W O 0.979(3) 0.646(3) 0.6635(17) 0.034(10) Uani 0.25 1 d PU
O15W O 0.821(2) 0.918(3) 0.9231(16) 0.031(10) Uani 0.25 1 d PU
N1 N 1.6142(12) 0.6972(13) 1.0172(8) 0.073(3) Uani 1 1 d U
N2 N 1.0254(13) 0.2822(15) 0.9374(9) 0.081(3) Uani 1 1 d U
C1 C 1.6401(15) 0.7290(16) 1.0709(9) 0.073(3) Uani 1 1 d U
H1A H 1.6645 0.7922 1.0728 0.110 Uiso 1 1 calc R
H1B H 1.6739 0.6805 1.0897 0.110 Uiso 1 1 calc R
H1C H 1.5986 0.7349 1.0846 0.110 Uiso 1 1 calc R
C2 C 1.6819(15) 0.6883(16) 1.0000(10) 0.073(3) Uani 1 1 d U
H2A H 1.7047 0.7524 1.0012 0.110 Uiso 1 1 calc R
H2B H 1.6693 0.6637 0.9660 0.110 Uiso 1 1 calc R
H2C H 1.7156 0.6431 1.0216 0.110 Uiso 1 1 calc R
C3 C 1.5660(14) 0.7685(16) 0.9886(10) 0.073(3) Uani 1 1 d U
H3A H 1.5914 0.8308 0.9900 0.110 Uiso 1 1 calc R
H3B H 1.5244 0.7769 1.0020 0.110 Uiso 1 1 calc R
H3C H 1.5493 0.7467 0.9542 0.110 Uiso 1 1 calc R
C4 C 1.5763(14) 0.5982(16) 1.0159(10) 0.072(3) Uani 1 1 d U
H4A H 1.5595 0.5753 0.9817 0.108 Uiso 1 1 calc R
H4B H 1.5349 0.6055 1.0296 0.108 Uiso 1 1 calc R
H4C H 1.6102 0.5508 1.0356 0.108 Uiso 1 1 calc R
C5 C 0.9628(15) 0.2900(18) 0.8873(11) 0.081(4) Uani 1 1 d U
H5A H 0.9166 0.2724 0.8934 0.122 Uiso 1 1 calc R
H5B H 0.9730 0.2455 0.8628 0.122 Uiso 1 1 calc R
H5C H 0.9602 0.3570 0.8748 0.122 Uiso 1 1 calc R
C6 C 1.0233(15) 0.1789(17) 0.9475(11) 0.081(4) Uani 1 1 d U
H6A H 1.0599 0.1634 0.9783 0.121 Uiso 1 1 calc R
H6B H 1.0331 0.1418 0.9203 0.121 Uiso 1 1 calc R
H6C H 0.9754 0.1616 0.9508 0.121 Uiso 1 1 calc R
C7 C 1.0942(15) 0.3111(18) 0.9227(11) 0.081(4) Uani 1 1 d U
H7A H 1.1359 0.3080 0.9518 0.121 Uiso 1 1 calc R
H7B H 1.0889 0.3777 0.9096 0.121 Uiso 1 1 calc R
H7C H 1.1014 0.2661 0.8975 0.121 Uiso 1 1 calc R
C8 C 1.0058(15) 0.3547(17) 0.9700(11) 0.080(4) Uani 1 1 d U
H8A H 1.0419 0.3542 1.0022 0.120 Uiso 1 1 calc R
H8B H 0.9583 0.3387 0.9744 0.120 Uiso 1 1 calc R
H8C H 1.0041 0.4196 0.9552 0.120 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O33 Nd1 O32 73.9(4) . .
O33 Nd1 O34 123.3(4) . .
O32 Nd1 O34 78.7(4) . .
O33 Nd1 O35 78.3(4) . .
O32 Nd1 O35 126.5(4) . .
O34 Nd1 O35 79.9(4) . .
O33 Nd1 O1W' 94.1(8) . .
O32 Nd1 O1W' 140.7(8) . .
O34 Nd1 O1W' 135.1(8) . .
O35 Nd1 O1W' 85.2(8) . .
O33 Nd1 O3W 133.3(4) . .
O32 Nd1 O3W 78.2(4) . .
O34 Nd1 O3W 85.9(5) . .
O35 Nd1 O3W 147.3(4) . .
O1W' Nd1 O3W 84.4(9) . .
O33 Nd1 O4 146.7(4) . 2_546
O32 Nd1 O4 138.9(4) . 2_546
O34 Nd1 O4 71.5(4) . 2_546
O35 Nd1 O4 75.4(4) . 2_546
O1W' Nd1 O4 63.8(8) . 2_546
O3W Nd1 O4 72.2(4) . 2_546
O33 Nd1 O1W 79.4(7) . .
O32 Nd1 O1W 143.2(6) . .
O34 Nd1 O1W 137.9(7) . .
O35 Nd1 O1W 70.2(7) . .
O1W' Nd1 O1W 19.3(8) . .
O3W Nd1 O1W 103.6(8) . .
O4 Nd1 O1W 72.8(7) 2_546 .
O33 Nd1 O2W 67.6(4) . .
O32 Nd1 O2W 73.9(4) . .
O34 Nd1 O2W 145.9(5) . .
O35 Nd1 O2W 133.1(4) . .
O1W' Nd1 O2W 67.0(8) . .
O3W Nd1 O2W 69.1(5) . .
O4 Nd1 O2W 118.9(4) 2_546 .
O1W Nd1 O2W 72.7(7) . .
O5W Nd2 O8W 122.3(13) . .
O5W Nd2 O2 133.9(10) . .
O8W Nd2 O2 76.8(9) . .
O5W Nd2 O4W' 153.8(13) . .
O8W Nd2 O4W' 68.8(19) . .
O2 Nd2 O4W' 69.4(11) . .
O5W Nd2 O4W 138.4(17) . .
O8W Nd2 O4W 84.7(18) . .
O2 Nd2 O4W 79.0(16) . .
O4W' Nd2 O4W 17.3(16) . .
O5W Nd2 O6W 93.4(12) . .
O8W Nd2 O6W 143.9(10) . .
O2 Nd2 O6W 73.9(6) . .
O4W' Nd2 O6W 81.4(18) . .
O4W Nd2 O6W 69.5(17) . .
O5W Nd2 O7W 68.7(11) . .
O8W Nd2 O7W 118.5(12) . .
O2 Nd2 O7W 65.6(7) . .
O4W' Nd2 O7W 130.1(15) . .
O4W Nd2 O7W 129.3(18) . .
O6W Nd2 O7W 66.6(10) . .
O5W Nd2 O9W 85.1(11) . .
O8W Nd2 O9W 55.6(12) . .
O2 Nd2 O9W 72.5(9) . .
O4W' Nd2 O9W 117.7(17) . .
O4W Nd2 O9W 135.0(17) . .
O6W Nd2 O9W 130.8(10) . .
O7W Nd2 O9W 67.2(12) . .
O39 Ge1 O37 112.2(5) . .
O39 Ge1 O36 110.5(5) . .
O37 Ge1 O36 107.6(4) . .
O39 Ge1 O38 111.0(5) . .
O37 Ge1 O38 107.8(5) . .
O36 Ge1 O38 107.4(5) . .
O1 W1 O14 100.8(6) . .
O1 W1 O18 102.5(5) . .
O14 W1 O18 90.6(5) . .
O1 W1 O19 101.8(6) . .
O14 W1 O19 157.4(5) . .
O18 W1 O19 85.3(5) . .
O1 W1 O27 98.9(5) . .
O14 W1 O27 89.4(5) . .
O18 W1 O27 158.2(5) . .
O19 W1 O27 86.4(5) . .
O1 W1 O38 169.5(5) . .
O14 W1 O38 72.9(4) . .
O18 W1 O38 86.3(4) . .
O19 W1 O38 84.6(4) . .
O27 W1 O38 72.9(4) . .
O2 W2 O32 103.6(5) . .
O2 W2 O20 101.9(5) . .
O32 W2 O20 94.3(5) . .
O2 W2 O21 100.2(5) . .
O32 W2 O21 91.2(5) . .
O20 W2 O21 155.3(5) . .
O2 W2 O14 92.9(5) . .
O32 W2 O14 163.3(5) . .
O20 W2 O14 84.6(5) . .
O21 W2 O14 83.4(5) . .
O2 W2 O38 164.4(5) . .
O32 W2 O38 91.4(4) . .
O20 W2 O38 72.4(4) . .
O21 W2 O38 83.4(4) . .
O14 W2 O38 72.3(4) . .
O3 W3 O30 103.6(5) . .
O3 W3 O20 98.4(5) . .
O30 W3 O20 90.3(5) . .
O3 W3 O31 101.2(5) . .
O30 W3 O31 86.9(5) . .
O20 W3 O31 160.3(5) . .
O3 W3 O27 98.9(5) . .
O30 W3 O27 157.5(5) . .
O20 W3 O27 86.4(5) . .
O31 W3 O27 88.7(5) . .
O3 W3 O38 168.8(5) . .
O30 W3 O38 82.5(4) . .
O20 W3 O38 72.0(4) . .
O31 W3 O38 88.3(4) . .
O27 W3 O38 75.3(4) . .
O4 W4 O33 103.9(5) . .
O4 W4 O21 101.5(5) . .
O33 W4 O21 94.2(5) . .
O4 W4 O16 98.3(5) . .
O33 W4 O16 90.3(5) . .
O21 W4 O16 158.0(4) . .
O4 W4 O24 93.7(5) . .
O33 W4 O24 161.9(5) . .
O21 W4 O24 86.2(5) . .
O16 W4 O24 83.0(4) . .
O4 W4 O36 163.8(4) . .
O33 W4 O36 89.9(4) . .
O21 W4 O36 85.6(4) . .
O16 W4 O36 72.9(4) . .
O24 W4 O36 72.1(4) . .
O5 W5 O17 102.3(6) . .
O5 W5 O15 102.4(5) . .
O17 W5 O15 86.2(5) . .
O5 W5 O16 98.4(5) . .
O17 W5 O16 91.1(4) . .
O15 W5 O16 159.1(5) . .
O5 W5 O28 101.1(5) . .
O17 W5 O28 156.5(5) . .
O15 W5 O28 86.7(5) . .
O16 W5 O28 87.6(5) . .
O5 W5 O36 169.6(4) . .
O17 W5 O36 83.2(4) . .
O15 W5 O36 86.7(4) . .
O16 W5 O36 72.4(4) . .
O28 W5 O36 74.1(4) . .
O6 W6 O24 102.2(6) . .
O6 W6 O28 100.3(5) . .
O24 W6 O28 90.3(5) . .
O6 W6 O18 101.5(6) . .
O24 W6 O18 89.8(5) . .
O28 W6 O18 157.6(4) . .
O6 W6 O26 100.8(6) . .
O24 W6 O26 157.0(5) . .
O28 W6 O26 86.9(5) . .
O18 W6 O26 84.3(5) . .
O6 W6 O36 171.3(5) . .
O24 W6 O36 72.6(4) . .
O28 W6 O36 73.0(4) . .
O18 W6 O36 85.6(4) . .
O26 W6 O36 84.8(4) . .
O7 W7 O26 103.2(6) . .
O7 W7 O19 102.2(6) . .
O26 W7 O19 86.4(5) . .
O7 W7 O22 97.8(6) . .
O26 W7 O22 159.0(5) . .
O19 W7 O22 88.6(5) . .
O7 W7 O23 100.0(6) . .
O26 W7 O23 88.6(5) . .
O19 W7 O23 157.9(5) . .
O22 W7 O23 88.4(5) . .
O7 W7 O37 169.3(6) . .
O26 W7 O37 84.8(4) . .
O19 W7 O37 85.2(4) . .
O22 W7 O37 74.5(4) . .
O23 W7 O37 72.9(4) . .
O8 W8 O25 104.1(6) . .
O8 W8 O31 100.2(6) . .
O25 W8 O31 88.3(5) . .
O8 W8 O13 99.0(6) . .
O25 W8 O13 91.5(5) . .
O31 W8 O13 160.2(5) . .
O8 W8 O22 99.5(6) . .
O25 W8 O22 156.3(4) . .
O31 W8 O22 85.8(5) . .
O13 W8 O22 86.6(5) . .
O8 W8 O37 169.9(5) . .
O25 W8 O37 83.8(4) . .
O31 W8 O37 86.2(4) . .
O13 W8 O37 74.2(4) . .
O22 W8 O37 73.0(4) . .
O9 W9 O12 103.4(6) . .
O9 W9 O15 101.6(6) . .
O12 W9 O15 87.8(5) . .
O9 W9 O13 98.0(6) . .
O12 W9 O13 91.7(5) . .
O15 W9 O13 159.9(5) . .
O9 W9 O23 99.2(6) . .
O12 W9 O23 157.3(5) . .
O15 W9 O23 87.2(5) . .
O13 W9 O23 85.7(5) . .
O9 W9 O37 169.1(6) . .
O12 W9 O37 84.9(4) . .
O15 W9 O37 85.5(4) . .
O13 W9 O37 74.4(4) . .
O23 W9 O37 72.7(4) . .
O10 W10 O34 101.3(5) . .
O10 W10 O29 98.9(5) . .
O34 W10 O29 95.2(5) . .
O10 W10 O30 101.7(5) . .
O34 W10 O30 94.4(5) . .
O29 W10 O30 155.0(4) . .
O10 W10 O25 92.9(5) . .
O34 W10 O25 165.4(4) . .
O29 W10 O25 85.5(4) . .
O30 W10 O25 79.5(4) . .
O10 W10 O39 170.5(5) . .
O34 W10 O39 83.4(4) . .
O29 W10 O39 72.3(4) . .
O30 W10 O39 86.0(4) . .
O25 W10 O39 83.0(4) . .
O11 W11 O35 100.9(5) . .
O11 W11 O29 99.8(5) . .
O35 W11 O29 95.2(5) . .
O11 W11 O17 102.1(5) . .
O35 W11 O17 94.4(5) . .
O29 W11 O17 153.9(5) . .
O11 W11 O12 92.6(5) . .
O35 W11 O12 166.3(5) . .
O29 W11 O12 84.8(4) . .
O17 W11 O12 80.2(4) . .
O11 W11 O39 170.4(5) . .
O35 W11 O39 84.7(4) . .
O29 W11 O39 71.8(4) . .
O17 W11 O39 85.0(4) . .
O12 W11 O39 82.2(4) . .
W2 O2 Nd2 157.2(7) . .
W4 O4 Nd1 153.5(6) . 2_556
W9 O12 W11 154.5(6) . .
W8 O13 W9 118.5(6) . .
W1 O14 W2 120.2(6) . .
W5 O15 W9 149.0(6) . .
W5 O16 W4 118.9(5) . .
W5 O17 W11 156.8(7) . .
W1 O18 W6 153.6(6) . .
W7 O19 W1 151.4(7) . .
W3 O20 W2 120.6(6) . .
W4 O21 W2 145.6(6) . .
W7 O22 W8 118.8(5) . .
W7 O23 W9 120.0(5) . .
W6 O24 W4 120.5(5) . .
W8 O25 W10 155.3(6) . .
W7 O26 W6 152.7(7) . .
W3 O27 W1 119.6(6) . .
W6 O28 W5 121.0(5) . .
W10 O29 W11 119.2(5) . .
W3 O30 W10 156.7(6) . .
W8 O31 W3 147.3(6) . .
W2 O32 Nd1 158.0(6) . .
W4 O33 Nd1 154.4(7) . .
W10 O34 Nd1 128.6(5) . .
W11 O35 Nd1 126.1(5) . .
Ge1 O36 W4 121.4(5) . .
Ge1 O36 W5 121.7(5) . .
W4 O36 W5 95.6(4) . .
Ge1 O36 W6 123.7(5) . .
W4 O36 W6 94.9(3) . .
W5 O36 W6 91.9(3) . .
Ge1 O37 W9 121.0(5) . .
Ge1 O37 W7 126.0(5) . .
W9 O37 W7 94.5(4) . .
Ge1 O37 W8 120.9(5) . .
W9 O37 W8 92.6(4) . .
W7 O37 W8 93.7(3) . .
Ge1 O38 W2 122.5(5) . .
Ge1 O38 W3 121.7(5) . .
W2 O38 W3 94.8(4) . .
Ge1 O38 W1 123.1(5) . .
W2 O38 W1 94.5(4) . .
W3 O38 W1 92.3(4) . .
Ge1 O39 W10 122.4(5) . .
Ge1 O39 W11 123.5(5) . .
W10 O39 W11 96.0(4) . .
O1W' O1W Nd1 76(3) . .
O1W O1W' Nd1 85(3) . .
O4W' O4W Nd2 77(7) . .
O4W O4W' Nd2 86(7) . .
C3 N1 C2 111(2) . .
C3 N1 C1 110(2) . .
C2 N1 C1 105(2) . .
C3 N1 C4 111(2) . .
C2 N1 C4 111.5(19) . .
C1 N1 C4 107.6(19) . .
C6 N2 C8 121(2) . .
C6 N2 C7 112(2) . .
C8 N2 C7 112(2) . .
C6 N2 C5 101(2) . .
C8 N2 C5 104(2) . .
C7 N2 C5 104(2) . .
N1 C1 H1A 109.5 . .
N1 C1 H1B 109.5 . .
H1A C1 H1B 109.5 . .
N1 C1 H1C 109.5 . .
H1A C1 H1C 109.5 . .
H1B C1 H1C 109.5 . .
N1 C2 H2A 109.5 . .
N1 C2 H2B 109.5 . .
H2A C2 H2B 109.5 . .
N1 C2 H2C 109.5 . .
H2A C2 H2C 109.5 . .
H2B C2 H2C 109.5 . .
N1 C3 H3A 109.5 . .
N1 C3 H3B 109.5 . .
H3A C3 H3B 109.5 . .
N1 C3 H3C 109.5 . .
H3A C3 H3C 109.5 . .
H3B C3 H3C 109.5 . .
N1 C4 H4A 109.5 . .
N1 C4 H4B 109.5 . .
H4A C4 H4B 109.5 . .
N1 C4 H4C 109.5 . .
H4A C4 H4C 109.5 . .
H4B C4 H4C 109.5 . .
N2 C5 H5A 109.5 . .
N2 C5 H5B 109.5 . .
H5A C5 H5B 109.5 . .
N2 C5 H5C 109.5 . .
H5A C5 H5C 109.5 . .
H5B C5 H5C 109.5 . .
N2 C6 H6A 109.5 . .
N2 C6 H6B 109.5 . .
H6A C6 H6B 109.5 . .
N2 C6 H6C 109.5 . .
H6A C6 H6C 109.5 . .
H6B C6 H6C 109.5 . .
N2 C7 H7A 109.5 . .
N2 C7 H7B 109.5 . .
H7A C7 H7B 109.5 . .
N2 C7 H7C 109.5 . .
H7A C7 H7C 109.5 . .
H7B C7 H7C 109.5 . .
N2 C8 H8A 109.5 . .
N2 C8 H8B 109.5 . .
H8A C8 H8B 109.5 . .
N2 C8 H8C 109.5 . .
H8A C8 H8C 109.5 . .
H8B C8 H8C 109.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Nd1 O33 2.387(10) .
Nd1 O32 2.387(12) .
Nd1 O34 2.420(10) .
Nd1 O35 2.448(11) .
Nd1 O1W' 2.47(3) .
Nd1 O3W 2.474(13) .
Nd1 O4 2.500(10) 2_546
Nd1 O1W 2.54(3) .
Nd1 O2W 2.680(14) .
Nd2 O5W 2.38(3) .
Nd2 O8W 2.40(4) .
Nd2 O2 2.419(12) .
Nd2 O4W' 2.43(5) .
Nd2 O4W 2.50(7) .
Nd2 O6W 2.67(3) .
Nd2 O7W 2.70(3) .
Nd2 O9W 2.70(4) .
Ge1 O39 1.730(10) .
Ge1 O37 1.741(10) .
Ge1 O36 1.742(9) .
Ge1 O38 1.743(10) .
W1 O1 1.729(12) .
W1 O14 1.879(12) .
W1 O18 1.906(11) .
W1 O19 1.931(12) .
W1 O27 1.957(11) .
W1 O38 2.381(10) .
W2 O2 1.723(12) .
W2 O32 1.763(12) .
W2 O20 1.935(11) .
W2 O21 1.940(11) .
W2 O14 2.064(13) .
W2 O38 2.274(10) .
W3 O3 1.716(11) .
W3 O30 1.897(12) .
W3 O20 1.934(11) .
W3 O31 1.939(12) .
W3 O27 1.942(11) .
W3 O38 2.291(10) .
W4 O4 1.752(10) .
W4 O33 1.761(11) .
W4 O21 1.917(12) .
W4 O16 1.980(11) .
W4 O24 2.063(11) .
W4 O36 2.240(9) .
W5 O5 1.720(12) .
W5 O17 1.902(11) .
W5 O15 1.911(11) .
W5 O16 1.928(10) .
W5 O28 1.950(11) .
W5 O36 2.301(11) .
W6 O6 1.701(12) .
W6 O24 1.852(11) .
W6 O28 1.909(12) .
W6 O18 1.926(12) .
W6 O26 1.939(12) .
W6 O36 2.373(10) .
W7 O7 1.696(13) .
W7 O26 1.900(12) .
W7 O19 1.915(12) .
W7 O22 1.930(11) .
W7 O23 1.944(13) .
W7 O37 2.300(10) .
W8 O8 1.719(11) .
W8 O25 1.803(11) .
W8 O31 1.903(12) .
W8 O13 1.936(12) .
W8 O22 1.986(11) .
W8 O37 2.322(9) .
W9 O9 1.727(13) .
W9 O12 1.799(11) .
W9 O15 1.930(11) .
W9 O13 1.953(11) .
W9 O23 1.956(12) .
W9 O37 2.299(11) .
W10 O10 1.722(10) .
W10 O34 1.762(11) .
W10 O29 1.925(12) .
W10 O30 1.953(12) .
W10 O25 2.089(11) .
W10 O39 2.229(9) .
W11 O11 1.733(12) .
W11 O35 1.785(11) .
W11 O29 1.929(11) .
W11 O17 1.949(10) .
W11 O12 2.091(11) .
W11 O39 2.244(11) .
O4 Nd1 2.500(10) 2_556
O1W O1W' 0.84(3) .
O4W O4W' 0.75(7) .
N1 C3 1.41(3) .
N1 C2 1.48(3) .
N1 C1 1.49(3) .
N1 C4 1.51(3) .
N2 C6 1.42(3) .
N2 C8 1.44(3) .
N2 C7 1.51(3) .
N2 C5 1.56(3) .
C1 H1A 0.9600 .
C1 H1B 0.9600 .
C1 H1C 0.9600 .
C2 H2A 0.9600 .
C2 H2B 0.9600 .
C2 H2C 0.9600 .
C3 H3A 0.9600 .
C3 H3B 0.9600 .
C3 H3C 0.9600 .
C4 H4A 0.9600 .
C4 H4B 0.9600 .
C4 H4C 0.9600 .
C5 H5A 0.9600 .
C5 H5B 0.9600 .
C5 H5C 0.9600 .
C6 H6A 0.9600 .
C6 H6B 0.9600 .
C6 H6C 0.9600 .
C7 H7A 0.9600 .
C7 H7B 0.9600 .
C7 H7C 0.9600 .
C8 H8A 0.9600 .
C8 H8B 0.9600 .
C8 H8C 0.9600 .
